#------------------------------------------------------------------------------
#$Date: 2021-04-30 11:19:27 +0300 (Fri, 30 Apr 2021) $
#$Revision: 264720 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/23/1562308.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562308
loop_
_publ_author_name
'Li, Na'
'Mu, Bao'
'Cao, Xinyu'
'Huang, Rudan'
_publ_section_title
;
 The structures and properties of the new two-dimensional
 inorganic--organic hybrid materials based on the molybdate chains
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              180
_journal_page_last               186
_journal_paper_doi               10.1016/j.jssc.2014.06.001
_journal_volume                  217
_journal_year                    2014
_chemical_formula_sum            'C16 H20 Cu Mo6 N6 O22'
_chemical_formula_weight         1287.56
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                105.551(2)
_cell_angle_beta                 92.0130(10)
_cell_angle_gamma                99.0090(10)
_cell_formula_units_Z            1
_cell_length_a                   7.5755(6)
_cell_length_b                   9.9208(8)
_cell_length_c                   10.2918(9)
_cell_measurement_reflns_used    2170
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      27.964
_cell_measurement_theta_min      3.287
_cell_volume                     733.55(11)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.974
_diffrn_measured_fraction_theta_max 0.974
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0409
_diffrn_reflns_av_sigmaI/netI    0.0725
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            3581
_diffrn_reflns_theta_full        25.02
_diffrn_reflns_theta_max         25.02
_diffrn_reflns_theta_min         3.29
_exptl_absorpt_coefficient_mu    3.300
_exptl_absorpt_correction_T_max  0.5174
_exptl_absorpt_correction_T_min  0.3519
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_density_diffrn    2.915
_exptl_crystal_density_meas      0
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             615
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.23
_refine_diff_density_max         3.290
_refine_diff_density_min         -2.945
_refine_diff_density_rms         0.494
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.056
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     232
_refine_ls_number_reflns         2520
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.056
_refine_ls_R_factor_all          0.0826
_refine_ls_R_factor_gt           0.0722
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1320P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1779
_refine_ls_wR_factor_ref         0.1883
_reflns_number_gt                2047
_reflns_number_total             2520
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2014-217-180.cif
_cod_data_source_block           3
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Triclinic' was changed to
'triclinic' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_cell_volume        733.55(10)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               1562308
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.19928(12) -0.19342(9) 0.36542(9) 0.0162(3) Uani 1 1 d . . .
Mo2 Mo 0.50129(11) -0.09070(9) 0.62239(9) 0.0141(3) Uani 1 1 d . . .
Mo3 Mo -0.00133(11) 0.07590(9) 0.36222(9) 0.0156(3) Uani 1 1 d . . .
Cu1 Cu 0.5000 0.0000 1.0000 0.0193(5) Uani 1 2 d S . .
N1 N 0.3977(13) 0.2336(9) 0.9033(9) 0.022(2) Uani 1 1 d . . .
H1 H 0.4332 0.1966 0.8253 0.027 Uiso 1 1 calc R . .
N2 N 0.4108(13) 0.1831(10) 1.0101(9) 0.023(2) Uani 1 1 d . . .
N3 N 0.1927(13) 0.5579(10) 0.6473(9) 0.026(2) Uani 1 1 d . . .
H3 H 0.1613 0.5990 0.5887 0.031 Uiso 1 1 calc R . .
O1 O 0.4566(10) -0.1226(7) 0.4069(7) 0.0176(16) Uani 1 1 d . . .
O2 O 0.2427(9) -0.0907(8) 0.5892(7) 0.0189(16) Uani 1 1 d . . .
O3 O 0.2456(9) 0.0370(7) 0.3804(7) 0.0177(16) Uani 1 1 d . . .
O4 O -0.0170(10) -0.1266(7) 0.4156(8) 0.0184(16) Uani 1 1 d . . .
O5 O 0.1737(10) -0.3523(8) 0.4039(8) 0.0234(17) Uani 1 1 d . . .
O6 O 0.1863(11) -0.2381(8) 0.1929(7) 0.0240(17) Uani 1 1 d . . .
O7 O 0.4898(10) -0.0303(8) 0.7957(7) 0.0208(17) Uani 1 1 d . . .
O8 O 0.5031(10) -0.2652(7) 0.5964(8) 0.0211(17) Uani 1 1 d . . .
O9 O 0.0730(10) 0.2473(8) 0.3672(8) 0.0271(19) Uani 1 1 d . . .
O10 O -0.0509(11) -0.0066(9) 0.1959(8) 0.0287(19) Uani 1 1 d . . .
O11 O 0.2215(12) -0.1058(8) 0.9872(8) 0.032(2) Uani 1 1 d . . .
H11B H 0.1480 -0.0610 0.9595 0.039 Uiso 1 1 d R . .
H11C H 0.1911 -0.1225 1.0608 0.039 Uiso 1 1 d R . .
C1 C 0.3458(17) 0.2689(12) 1.1094(12) 0.028(3) Uani 1 1 d . . .
H1A H 0.3398 0.2598 1.1968 0.034 Uiso 1 1 calc R . .
C2 C 0.2874(17) 0.3750(13) 1.0646(12) 0.029(3) Uani 1 1 d . . .
H2 H 0.2350 0.4488 1.1150 0.035 Uiso 1 1 calc R . .
C3 C 0.3213(15) 0.3505(11) 0.9342(11) 0.023(2) Uani 1 1 d . . .
C4 C 0.2808(16) 0.4527(12) 0.6100(12) 0.026(3) Uani 1 1 d . . .
H4 H 0.3118 0.4247 0.5213 0.032 Uiso 1 1 calc R . .
C5 C 0.3280(16) 0.3832(12) 0.7018(11) 0.027(3) Uani 1 1 d . . .
H5 H 0.3933 0.3098 0.6753 0.032 Uiso 1 1 calc R . .
C6 C 0.2797(15) 0.4215(11) 0.8314(11) 0.023(2) Uani 1 1 d . . .
C7 C 0.1900(17) 0.5382(12) 0.8678(12) 0.027(3) Uani 1 1 d . . .
H7 H 0.1586 0.5701 0.9560 0.033 Uiso 1 1 calc R . .
C8 C 0.1500(18) 0.6031(13) 0.7756(13) 0.034(3) Uani 1 1 d . . .
H8 H 0.0918 0.6809 0.8004 0.041 Uiso 1 1 calc R . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O6 Mo1 O5 104.6(4) . .
O6 Mo1 O4 105.7(4) . .
O5 Mo1 O4 103.1(3) . .
O6 Mo1 O1 100.5(3) . .
O5 Mo1 O1 102.7(3) . .
O4 Mo1 O1 136.9(3) . .
O6 Mo1 O3 92.0(3) . .
O5 Mo1 O3 163.3(3) . .
O4 Mo1 O3 73.1(3) . .
O1 Mo1 O3 72.4(3) . .
O6 Mo1 O2 168.2(3) . .
O5 Mo1 O2 86.6(3) . .
O4 Mo1 O2 74.6(3) . .
O1 Mo1 O2 73.0(3) . .
O3 Mo1 O2 76.8(3) . .
O8 Mo2 O7 103.3(4) . .
O8 Mo2 O3 95.8(3) . 2_656
O7 Mo2 O3 97.6(3) . 2_656
O8 Mo2 O2 101.2(3) . .
O7 Mo2 O2 91.3(3) . .
O3 Mo2 O2 158.4(3) 2_656 .
O8 Mo2 O1 90.1(3) . .
O7 Mo2 O1 162.2(3) . .
O3 Mo2 O1 92.3(3) 2_656 .
O2 Mo2 O1 74.5(3) . .
O8 Mo2 O1 160.7(3) . 2_656
O7 Mo2 O1 94.3(3) . 2_656
O3 Mo2 O1 73.8(3) 2_656 2_656
O2 Mo2 O1 86.0(3) . 2_656
O1 Mo2 O1 74.4(3) . 2_656
O10 Mo3 O9 104.0(4) . .
O10 Mo3 O2 97.8(4) . 2_556
O9 Mo3 O2 99.1(3) . 2_556
O10 Mo3 O3 98.8(3) . .
O9 Mo3 O3 92.5(3) . .
O2 Mo3 O3 156.8(3) 2_556 .
O10 Mo3 O4 163.5(3) . 2_556
O9 Mo3 O4 92.0(3) . 2_556
O2 Mo3 O4 75.1(3) 2_556 2_556
O3 Mo3 O4 84.6(3) . 2_556
O10 Mo3 O4 92.9(4) . .
O9 Mo3 O4 158.7(3) . .
O2 Mo3 O4 91.2(3) 2_556 .
O3 Mo3 O4 71.9(3) . .
O4 Mo3 O4 72.7(3) 2_556 .
N2 Cu1 N2 180.000(2) . 2_657
N2 Cu1 O7 93.6(3) . 2_657
N2 Cu1 O7 86.4(3) 2_657 2_657
N2 Cu1 O7 86.4(3) . .
N2 Cu1 O7 93.6(3) 2_657 .
O7 Cu1 O7 180.000(1) 2_657 .
N2 Cu1 O11 88.8(3) . .
N2 Cu1 O11 91.2(3) 2_657 .
O7 Cu1 O11 88.5(3) 2_657 .
O7 Cu1 O11 91.5(3) . .
N2 Cu1 O11 91.2(3) . 2_657
N2 Cu1 O11 88.8(3) 2_657 2_657
O7 Cu1 O11 91.5(3) 2_657 2_657
O7 Cu1 O11 88.5(3) . 2_657
O11 Cu1 O11 180.000(1) . 2_657
N2 N1 C3 110.7(9) . .
N2 N1 H1 124.7 . .
C3 N1 H1 124.7 . .
C1 N2 N1 106.6(9) . .
C1 N2 Cu1 130.8(8) . .
N1 N2 Cu1 122.5(7) . .
C4 N3 C8 121.3(10) . .
C4 N3 H3 119.3 . .
C8 N3 H3 119.3 . .
Mo1 O1 Mo2 104.9(3) . .
Mo1 O1 Mo2 105.3(3) . 2_656
Mo2 O1 Mo2 105.6(3) . 2_656
Mo3 O2 Mo2 155.9(4) 2_556 .
Mo3 O2 Mo1 102.0(3) 2_556 .
Mo2 O2 Mo1 101.2(3) . .
Mo2 O3 Mo3 150.5(4) 2_656 .
Mo2 O3 Mo1 105.8(3) 2_656 .
Mo3 O3 Mo1 102.6(3) . .
Mo1 O4 Mo3 104.6(3) . 2_556
Mo1 O4 Mo3 105.8(3) . .
Mo3 O4 Mo3 107.3(3) 2_556 .
Mo2 O7 Cu1 166.8(5) . .
Cu1 O11 H11B 112.5 . .
Cu1 O11 H11C 113.1 . .
H11B O11 H11C 110.3 . .
N2 C1 C2 109.7(10) . .
N2 C1 H1A 125.2 . .
C2 C1 H1A 125.2 . .
C3 C2 C1 106.4(10) . .
C3 C2 H2 126.8 . .
C1 C2 H2 126.8 . .
C2 C3 N1 106.7(10) . .
C2 C3 C6 131.6(11) . .
N1 C3 C6 121.6(10) . .
N3 C4 C5 120.1(11) . .
N3 C4 H4 120.0 . .
C5 C4 H4 120.0 . .
C6 C5 C4 120.4(11) . .
C6 C5 H5 119.8 . .
C4 C5 H5 119.8 . .
C5 C6 C7 117.3(10) . .
C5 C6 C3 123.7(10) . .
C7 C6 C3 119.0(10) . .
C8 C7 C6 119.8(11) . .
C8 C7 H7 120.1 . .
C6 C7 H7 120.1 . .
C7 C8 N3 121.0(12) . .
C7 C8 H8 119.5 . .
N3 C8 H8 119.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O6 1.706(7) .
Mo1 O5 1.710(7) .
Mo1 O4 1.899(7) .
Mo1 O1 1.956(7) .
Mo1 O3 2.220(7) .
Mo1 O2 2.244(7) .
Mo2 O8 1.682(7) .
Mo2 O7 1.733(7) .
Mo2 O3 1.911(7) 2_656
Mo2 O2 1.976(7) .
Mo2 O1 2.161(7) .
Mo2 O1 2.193(7) 2_656
Mo3 O10 1.688(8) .
Mo3 O9 1.692(7) .
Mo3 O2 1.930(7) 2_556
Mo3 O3 1.981(7) .
Mo3 O4 2.200(7) 2_556
Mo3 O4 2.207(7) .
Cu1 N2 2.013(9) .
Cu1 N2 2.013(9) 2_657
Cu1 O7 2.040(7) 2_657
Cu1 O7 2.040(7) .
Cu1 O11 2.187(8) .
Cu1 O11 2.187(8) 2_657
N1 N2 1.331(13) .
N1 C3 1.344(14) .
N1 H1 0.8600 .
N2 C1 1.308(14) .
N3 C4 1.305(15) .
N3 C8 1.344(15) .
N3 H3 0.8600 .
O1 Mo2 2.193(7) 2_656
O2 Mo3 1.930(7) 2_556
O3 Mo2 1.911(7) 2_656
O4 Mo3 2.200(7) 2_556
O11 H11B 0.8500 .
O11 H11C 0.8500 .
C1 C2 1.381(16) .
C1 H1A 0.9300 .
C2 C3 1.340(16) .
C2 H2 0.9300 .
C3 C6 1.469(15) .
C4 C5 1.378(16) .
C4 H4 0.9300 .
C5 C6 1.365(15) .
C5 H5 0.9300 .
C6 C7 1.406(16) .
C7 C8 1.332(17) .
C7 H7 0.9300 .
C8 H8 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
C3 N1 N2 C1 -1.1(13) . . . .
C3 N1 N2 Cu1 175.0(8) . . . .
N2 Cu1 N2 C1 76(100) 2_657 . . .
O7 Cu1 N2 C1 -13.5(11) 2_657 . . .
O7 Cu1 N2 C1 166.5(11) . . . .
O11 Cu1 N2 C1 74.9(11) . . . .
O11 Cu1 N2 C1 -105.1(11) 2_657 . . .
N2 Cu1 N2 N1 -99(100) 2_657 . . .
O7 Cu1 N2 N1 171.5(8) 2_657 . . .
O7 Cu1 N2 N1 -8.5(8) . . . .
O11 Cu1 N2 N1 -100.1(9) . . . .
O11 Cu1 N2 N1 79.9(9) 2_657 . . .
O6 Mo1 O1 Mo2 -171.7(3) . . . .
O5 Mo1 O1 Mo2 -64.0(4) . . . .
O4 Mo1 O1 Mo2 61.4(6) . . . .
O3 Mo1 O1 Mo2 99.5(3) . . . .
O2 Mo1 O1 Mo2 18.4(3) . . . .
O6 Mo1 O1 Mo2 77.1(4) . . . 2_656
O5 Mo1 O1 Mo2 -175.1(3) . . . 2_656
O4 Mo1 O1 Mo2 -49.8(6) . . . 2_656
O3 Mo1 O1 Mo2 -11.6(3) . . . 2_656
O2 Mo1 O1 Mo2 -92.7(3) . . . 2_656
O8 Mo2 O1 Mo1 80.7(4) . . . .
O7 Mo2 O1 Mo1 -59.1(11) . . . .
O3 Mo2 O1 Mo1 176.6(3) 2_656 . . .
O2 Mo2 O1 Mo1 -20.8(3) . . . .
O1 Mo2 O1 Mo1 -110.9(4) 2_656 . . .
O8 Mo2 O1 Mo2 -168.3(4) . . . 2_656
O7 Mo2 O1 Mo2 51.8(11) . . . 2_656
O3 Mo2 O1 Mo2 -72.5(3) 2_656 . . 2_656
O2 Mo2 O1 Mo2 90.1(3) . . . 2_656
O1 Mo2 O1 Mo2 0.0 2_656 . . 2_656
O8 Mo2 O2 Mo3 94.9(10) . . . 2_556
O7 Mo2 O2 Mo3 -9.0(10) . . . 2_556
O3 Mo2 O2 Mo3 -123.8(10) 2_656 . . 2_556
O1 Mo2 O2 Mo3 -178.1(10) . . . 2_556
O1 Mo2 O2 Mo3 -103.1(10) 2_656 . . 2_556
O8 Mo2 O2 Mo1 -69.2(3) . . . .
O7 Mo2 O2 Mo1 -173.1(3) . . . .
O3 Mo2 O2 Mo1 72.1(9) 2_656 . . .
O1 Mo2 O2 Mo1 17.8(3) . . . .
O1 Mo2 O2 Mo1 92.7(3) 2_656 . . .
O6 Mo1 O2 Mo3 108.9(16) . . . 2_556
O5 Mo1 O2 Mo3 -89.0(4) . . . 2_556
O4 Mo1 O2 Mo3 15.6(3) . . . 2_556
O1 Mo1 O2 Mo3 166.7(4) . . . 2_556
O3 Mo1 O2 Mo3 91.3(3) . . . 2_556
O6 Mo1 O2 Mo2 -77.7(17) . . . .
O5 Mo1 O2 Mo2 84.5(4) . . . .
O4 Mo1 O2 Mo2 -171.0(4) . . . .
O1 Mo1 O2 Mo2 -19.9(3) . . . .
O3 Mo1 O2 Mo2 -95.2(3) . . . .
O10 Mo3 O3 Mo2 91.8(9) . . . 2_656
O9 Mo3 O3 Mo2 -12.8(9) . . . 2_656
O2 Mo3 O3 Mo2 -133.1(8) 2_556 . . 2_656
O4 Mo3 O3 Mo2 -104.5(8) 2_556 . . 2_656
O4 Mo3 O3 Mo2 -178.0(9) . . . 2_656
O10 Mo3 O3 Mo1 -72.2(4) . . . .
O9 Mo3 O3 Mo1 -176.8(3) . . . .
O2 Mo3 O3 Mo1 62.9(8) 2_556 . . .
O4 Mo3 O3 Mo1 91.5(3) 2_556 . . .
O4 Mo3 O3 Mo1 18.0(3) . . . .
O6 Mo1 O3 Mo2 -86.9(4) . . . 2_656
O5 Mo1 O3 Mo2 88.5(11) . . . 2_656
O4 Mo1 O3 Mo2 167.3(4) . . . 2_656
O1 Mo1 O3 Mo2 13.4(3) . . . 2_656
O2 Mo1 O3 Mo2 89.5(3) . . . 2_656
O6 Mo1 O3 Mo3 85.0(4) . . . .
O5 Mo1 O3 Mo3 -99.7(11) . . . .
O4 Mo1 O3 Mo3 -20.9(3) . . . .
O1 Mo1 O3 Mo3 -174.7(4) . . . .
O2 Mo1 O3 Mo3 -98.6(3) . . . .
O6 Mo1 O4 Mo3 178.5(3) . . . 2_556
O5 Mo1 O4 Mo3 68.9(4) . . . 2_556
O1 Mo1 O4 Mo3 -56.3(6) . . . 2_556
O3 Mo1 O4 Mo3 -94.3(3) . . . 2_556
O2 Mo1 O4 Mo3 -13.8(3) . . . 2_556
O6 Mo1 O4 Mo3 -68.3(4) . . . .
O5 Mo1 O4 Mo3 -177.9(3) . . . .
O1 Mo1 O4 Mo3 56.9(6) . . . .
O3 Mo1 O4 Mo3 18.9(3) . . . .
O2 Mo1 O4 Mo3 99.4(3) . . . .
O10 Mo3 O4 Mo1 76.9(4) . . . .
O9 Mo3 O4 Mo1 -65.9(10) . . . .
O2 Mo3 O4 Mo1 174.7(3) 2_556 . . .
O3 Mo3 O4 Mo1 -21.4(3) . . . .
O4 Mo3 O4 Mo1 -111.3(5) 2_556 . . .
O10 Mo3 O4 Mo3 -171.8(4) . . . 2_556
O9 Mo3 O4 Mo3 45.4(10) . . . 2_556
O2 Mo3 O4 Mo3 -74.0(3) 2_556 . . 2_556
O3 Mo3 O4 Mo3 89.9(3) . . . 2_556
O4 Mo3 O4 Mo3 0.0 2_556 . . 2_556
O8 Mo2 O7 Cu1 22(2) . . . .
O3 Mo2 O7 Cu1 -75.8(19) 2_656 . . .
O2 Mo2 O7 Cu1 123.9(19) . . . .
O1 Mo2 O7 Cu1 160.6(14) . . . .
O1 Mo2 O7 Cu1 -150.0(19) 2_656 . . .
N2 Cu1 O7 Mo2 177.2(19) . . . .
N2 Cu1 O7 Mo2 -2.8(19) 2_657 . . .
O7 Cu1 O7 Mo2 -122(100) 2_657 . . .
O11 Cu1 O7 Mo2 -94.1(19) . . . .
O11 Cu1 O7 Mo2 85.9(19) 2_657 . . .
N1 N2 C1 C2 1.0(14) . . . .
Cu1 N2 C1 C2 -174.6(8) . . . .
N2 C1 C2 C3 -0.5(15) . . . .
C1 C2 C3 N1 -0.1(14) . . . .
C1 C2 C3 C6 175.8(12) . . . .
N2 N1 C3 C2 0.7(13) . . . .
N2 N1 C3 C6 -175.7(10) . . . .
C8 N3 C4 C5 1.7(18) . . . .
N3 C4 C5 C6 1.5(18) . . . .
C4 C5 C6 C7 -3.4(17) . . . .
C4 C5 C6 C3 178.5(11) . . . .
C2 C3 C6 C5 178.8(12) . . . .
N1 C3 C6 C5 -5.8(18) . . . .
C2 C3 C6 C7 1(2) . . . .
N1 C3 C6 C7 176.2(11) . . . .
C5 C6 C7 C8 2.4(18) . . . .
C3 C6 C7 C8 -179.5(12) . . . .
C6 C7 C8 N3 1(2) . . . .
C4 N3 C8 C7 -2.8(19) . . . .
